Foundations of Materials Science and Engineering Third Edition
Foundations of Materials Science and Engineering Third Edition
Production of Iron and Steel
Production of pig iron
Fe2O3 + 3CO
2Fe + 3CO2
After A. G. Guy,”Elements of Physical Metallurgy,”2nd ed., !959, Addision-Wesley, Fig. 2-5, p.21.
Pig iron and 30% steel crap is fed into refractory
furnace to which oxygen lane is inserted.
Oxygen reacts with liquid bath to form iron oxide.
FeO + C
Fe + CO
Slag forming fluxes
Carbon content and
other impurities are
Molten steel is
continuously cast and
formed into shapes.
Courtesy of Inland Steel
Iron Carbide Phase Diagram
Plain carbon steel
0.03% to 1.2% C, 0.25 to 1%
Mn and other impurities.
• α Ferrite: Very low solubility
of carbon. Max 0.02 % at 7230C
and 0.005% at 00C.
• Austenite: Interstitial solid
solution of carbon in γ
iron. Solubility of C is
2.08% at 11480C and 0.8%
• Cementite: Intermetallic compound.
6.67% C and 93.3% Fe.
Liquid (0.53%C) + δ (0.09% C)
γ austenite (2.08%C) + Fe3C ( 6.67%C)
γ Austenite (0.8%C)
γ (0.17% C)
Liquid (4.3% C) 1148 C
Less than 0.8%
α Ferrite(0.02%C) + Fe3C ( 6.67%C)
0.8% C More than 0.8% Hypereutectoid
Slow Cooling of Plain Carbon Steel
Eutectoid plain carbon steel: If a sample is heated up
to 7500C and held for sufficient time, structure will
become homogeneous austenite.
• Below eutectoid temperature,
layers of ferrite and cementite
After W. F. Smith, “The Structure and Properties of Engineering Alloys,” 2 nd ed.,McGraw-Hill, 1981, p.8
Slow Cooling of Plain Carbon Steel (Cont..)
• Hypoeutectoid plain carbon steel: If a sample of 0.4%
C is heated up to 9000C, it gets austenitized.
• Further cooling gives rise to α and pearlite.
After W. F. Smith, “The Structure and Properties of Engineering Alloys,” 2 nd ed.,McGraw-Hill, 1981, p.10
Slow Cooling of Plain Carbon Steel (Cont..)
Hypereutectoid plain carbon steel: If a 1.2% C sample
is heated up to 9500C and held for sufficient time, it
entirely gets austenitized.
• Further cooling results results in eutectoid cementite
After W. F. Smith, “The Structure and Properties of Engineering Alloys,” 2 nd ed.,McGraw-Hill, 1981, p.12.
Heat treatment of plain carbon steels.
Heating and cooling properties of steels vary
• Martensite: Metastable phase consisting of super
saturated solid solution of C in BCC or BCC tetragonal
• Caused by rapid cooling of austenitic steel into room
temperature of martensite start.
temperature of martensite finish.
Microstructure of Fe – C Martensites
Lath martensite: Less than 0.6% C and consists of
domains of lathe of different orientation.
• Plate martensite: More than 0.6% C and have fine
structure of parallel twins.
After A. R. Marder and G. Krauss, as presented in “Hardenebility Concepts with Applications to Steel,” AIME, 1978, p. 238.
Transfer to martensite is diffusionless.
No change of relative position of carbon atoms after
Strength and hardness increases
with carbon content.
• Strength is due to high dislocation
concentration and interstitial solid
9-11After E. R. Parker and V. F. Zackay
Strong and Ductile Steels, Sci.Am.,November 1968, p.36; Copyright by Scientific
Isothermal decomposition of Austenite.
Several samples are first austenitized above eutectoid temperature
and rapidly cooled in sand bath to desired temperature in a salt
bath and then quenched in water at various time intervals.
After W. F. Smith, “The Structure and Properties of Engineering Alloys,” McGraw-Hill, 1981, p.14
Isothermal decomposition of Austenite (Cont..)
If hot quenching temperature is between 5500C to
2500C, an intermediate structure Bainite is produced.
• Bainite contain nonlamellar eutectoid structure of α
ferrite and cementite.
• Upper Bainite
Between 5500C and 3500C
• Lower Bainite
Between 3500C and 2500C
After H. E. McGannon(ed.), “The Making Shaping and Treating of Steel,” 9 th ed., United States Steel Corp., 1971
IT Diagrams for Noneutectoid Steels
‘S’ curves of IT diagrams of noneutectoid steel is
shifted to left.
• Not possible to quench from austenitic region to
produce entirely martensite.
• Additional transformation
line indicates start and
formation of proeutectoid
After R. A. Grange, V. E. Lambert, and J. J. Harrington, Trans, ASM, 51:377(1959)
Continuous Cooling-Transformation Diagram
In continuous cooling transformation from martensite
to pearlite takes place at a range of temperature.
• Start and finish lines shifted to longer time.
• No transformation below 4500C.
After R. A. Grange and J. M. Kiefer, “Alloying Elements in Steel,” ASM 2 nd ed., 1966, p.254.
Annealing and Normalizing
Full annealing: Sample heated to 400C above austenite
ferrite boundary, held for necessary time and cooled
Process annealing: Used for stress
relief. Applied to hypoeutectoid
steel at eutectoid temperature.
Normalizing: Steel heated in
austenite region and cooled
in still air.
Makes grain structure
After T. G. Diggers et al., “ Heat Treatment and Properties of Iron and Steel,” NBS Monograph 88, 1966, p. 10
Tempering of Plain Carbon Steel
Martensitic steel is heated at a temperature below
• Makes steel softer and ductile.
• Carbon atoms, in low carbon
steels, segregate themselves on
200 – 7000C
400 – 7000C
From “ Suiting the heat Treatment to the job,” United States Steel Corp., 1968, p.34.
Effects of Tempering
Hardness decreases as temperature increases above
• This is due to diffusion of
carbon atoms from interstitial
sites to iron carbide precipitates.
After JE. C. Bain, and H. W. Paxton, “Alloying Elements in Steel, “ 2 nd ed., American Society for Metals, 1996 p.38.
Martempering and Austempering
Martempering (Marquenching): Austinitizing,
quenching at around Ms, holding in quenching media
until temperature is uniform, removing before Bainite
forms and cooling at a moderate rate.
• Austempering: Same as martempering but held at
quenching media till austenite to Bainite
transformation takes place.
Source: “Metals Handbook,” vol. 2, 8th ed., American Society for Metals, 1964.
Calssification of Plain Carbon Steel
Four digit AISI-SAE code.
First two digits, 10, indicate plain carbon
• Last two digits indicate carbon content in
• Example: 1030 steel indicate plain carbon
steel containing 0.30 wt% carbon.
• As carbon content increase, steel becomes
stronger and ductile.
Low Alloy Steels
Limitations of plain carbon steels:
Cannot be strengthened beyond 690 MPa without
loosing ductility and impact strength.
Not deep hardenable.
Low corrosion resistance
Rapid quenching leads to crack and distortion.
Poor impact resistance at low temperature.
• Alloy steels: Up to 50% alloying elements like
manganese, nickel, chromium, molybdenum and
Classification of Alloy Steels
First two digits: Principle alloying element.
Last two digits: % of carbon.
Source: “Alooy Steel: Semifinished; Hot-Rolled and Cold-Finished Bars,” American Iron and Steel Institute, 1970.
Distribution of Alloying Elements
Distribution depends upon compound and carbide
forming tendency of each element.
After JE. C. Bain, and H. W. Paxton, “Alloying Elements in Steel, “ 2 nd ed., American Society for Metals, 1996
Effects of Alloying Element on Eutectoid Temperature
Mn and Ni lower eutectoid temperature.
They act as austenite stabilizing
and titanium raise
They are called ferrite
Source: “Metals Handbook,” vol. 2, 9th ed., American Society for Metals, 1973.
• Hardenability determines the depth and distribution of
hardness induced by quenching.
• Hardenability depends on
Austenitic grain size
• Joming hardenability test:
Cylindrical bar (1 inch dia and 4
inch length with 1/16 in flange
at one end is austenitized and one
end is quenched.
Rockwell C hardness is measured
up to 2.5 inch from quenched end.
After H. E. McGannon(ed.), “The Making Shaping and Treating of Steel,” 9 th ed., United States Steel Corp., 1971, p.1099
• For 1080 plain carbon steel, the hardness value at
quenched end is 65 HRC while it is 50 HRC at 3/16
inch from quenched end.
• Alloy steel 4340 has high
hardenability and has
hardness of 40 HRC 2 inches
from quenched end.
• In alloy steel, decomposition
of austenite to ferrite is delayed.
• Cooling rate depends on bar dia,
quenching media and bar cross
After H. E. McGannon(ed.), “The Making Shaping and Treating of Steel,” United States Steel Corp., 1971, p.1139.
Mechanical Properties of Low Alloy Steels
Precipitation Strengthening : Creates fine dispersion of
precipitated particles in the metal and hinder
• Basic steps :
Solution heat treatment: Alloy sample
heated to a temperature between solvus and
solidus and soaked at that temperature.
Quenching: Sample then quenched to room
temperature in water.
Aging: Solutionized and quenched sample is
then aged to form finely dispersed particles.
Decomposition Products Created by Aging
• Super saturated solid solution is in unstable condition.
• Alloy tends to seek a lower
energy state by decomposing
into metastable or equilibrium
• Supersaturated solid solution
as highest energy state.
• Equilibrium precipitate has
lowest energy state.
Effects of Aging on Strength
• Aging curve: Plot of strength or hardness versus aging
• As aging time increases
alloy becomes stronger
harder and less ductile.
• Overaging decreases
strength and hardness.
Example - Al 4% Cu Alloy
• Al -4% Cu is solutionized at about 5150C
• Alloy is rapidly cooled in water.
• Alloy is artificially aged in 130 – 1900C
• Structures formed :
GP1 Zone: At lower aging temperature,
copper atom is segregated in supersaturated
GP2 Zone: Tetragonal structure, 10-100 nm
θ’ Phase: Nucleates heterogeneously on
θ Phase: Equilibrium phase, incoherent
Correlation of Structure and Hardness
GP1 and GP2 Zones increases hardness by stopping
• At 1300C when θ’ forms, hardness is maximum.
• After θ’ forms, GP2
zones are dissolved
and θ’ gets coarsened
After J. M. Silcock, T. J. Heal, and H. K. Hardy “Alluminium,” 1, American society of Metals, 1967,p.123.
General Properties of Aluminum
Low density, corrosion resistance.
High alloy strength (about 690 MPa)
Nontoxic and good electrical properties.
• Aluminum hydroxide is
precipitated from aluminum
• Aluminum hydroxide is
thickened and calcined to
Al2O3 which is dissolve in
cryolite and electrolyzed.
• Metallic aluminum sinks to bottom and is tapped out.
Courtesy of Aluminium Company of America
Wrought Aluminum Alloys
Primary Fabrication: Usually semiconsciously cast by
direct chill method.
Scalping: ½ inch metal is removed from hot rolled
surface for good finishing.
Ingots are homogenized and rolled.
Classification: According to
major alloying elements.
Four digits: First digit major group of alloying
Second digit: Impurity limits.
Last 2 digits: Identify
Temper designations are designated by hyphen.
F – as fabricated
O – Annealed
H – Strain hardened.
T – Heat treated to
H1 – Strain hardened
H2 – Strain hardened
H3 - Strain hardened
T1 – Naturally aged
T3 – Solution heat treated.
T4 – Solution heat treated
and naturally aged.
T5 - Cooled and artificially
T6 - Solution heat treated
and artificially aged.
T7 - Solution heat treated
T8 - Solution heat treated,
cold worked and then
Non Heat Treatable Aluminum Alloys
1xxx alloys : 99% Al + Fe + Si + 0.12% Cu
Tensile strength = 90 MPa
Used for sheet metals
3xxx alloys : Manganese is principle alloying element.
Al 3003 = Al 1100 + 1.25% Mn
Tensile strength = 110 MPa
General purpose alloy
5xxx alloys: Al + up to 5% Mg
Al5052 = Al + 25%Mg + 0.2% Cr
Tensile strength = 193 MPa
Used in bus, truck and marine sheet metals.
Heat Treatable Aluminum Alloys
• 2xxx alloys : Al + Cu + Mg
Al2024 = Al + 4.5% Cu + 1.5% Mg +0.6%Mn
Strength = 442 MPa
Used for aircraft structures.
• 6xxx alloys: Al + Mg + Si
Al6061 = Al + 1% Mg + 0.6%Si + 0.3% Cu + 0.2% Cr
Strength = 290 MPa
Used for general purpose structure.
• 7xxx alloys: A + Zn + Mg + Cu
Al7075 = Al + 5.6% Zn + 2.5% Mg + 1.6% Cu + 0.25% Cr
Strength = 504 MPa
Used for aircraft structures.
• Sand Casting: Simple and used for small
quantities and complex jobs.
• Permanent mold casting: Molten metal is
poured into permanent metal mold.
Finer grain structure and strength due to fast cooling.
Less shrinkage and porosity.
More shrinkage and simple parts only.
• Die casting: Molten metal forced into molds
Almost finished parts, automatic.
Good tolerance and surface finish.
Fine grain structure.
Aluminum Casting Alloy Composites
Composition of casting alloys differs greatly from
• Casting properties and
are of primary interest.
• Denoted as 4 digits
with a period between
last two digits.
General properties of Copper: Good electrical and
thermal conduction, ease of fabrication, corrosion
resistance, medium strength.
• Production of copper:
Copper sulfide concentrates are smelted.
Copper sulfide is converted to blister copper by
blowing air through matte.
Impurities in blister copper removed as slag in
tough pitch copper.
Tough pitch copper is further refined
Classification of Copper Alloys
Numbers C10100 to C79900 designate wrought alloys.
Numbers C80000 to C99900 designate casting alloys.
Electrolytic tough pitch copper is least expensive and
used in production of wire, rod, and strip.
Has 0.04% oxygen.
Cu2O + H2 Heated
2Cu + H2O
H2O causes inner holes and
Copper cast in controlled
Oxygen free high conductive
Courtesy of Amax Base Metals Research, Inc.
Copper Zinc Alloys
Copper forms substitutional solid solution with Zn till
• Cartridge brass 70% Cu & 30% Zn single phase
• Muntz brass
60% Cu & 40% Zn
• Zinc (0.5 to 3%) is always added to copper to increase
Courtesy of Anaconda American Brass Co
Other Copper Alloys
Copper-Tin Bronzes: 1 to 10% tin with Cu to form
solid solution strengthened alloys.
Stronger and less corrosive than Cu-Zn bronzes.
Up to 16% Sn is added to alloys that are used for
high strength bearings.
• Copper beryllium alloys: 0.6 to 2% Be and 0.2 – 2.5 %
Cobalt with copper.
Can be heat treated and cold worked to produce
very strong (1463 MPa) bronzes.
Excellent corrosion resistance and fatigue
Used in springs, diaphragms, valves etc.
Excellent corrosion resistance in stainless steel is due to
high (at least 12%) Chromium forming chromium
oxide on surface.
• Ferrite stainless steel :
Structure is mainly
ferritic (BCC α ).
Cr extends α region
and suppresses γ region
forming γ loop.
Low cost high strength (517 MPa) and hence used
in construction materials.
After “Metals Handbook,” vol. 8, 8th ed., American Society for Metals, 1973, p.291.
Martensitic Stainless Steel
12 – 17% Cr and 0.15 – 1% C.
Martensite formed from quenching from austenite
Poor corrosion resistance.
Heat treatment: Same as plain carbon steel.
Tensile strength : 517 MPa to 1966 MPa.
Used for machine parts, pumps, bearings, and valve
When carbon content is greater than 1%, α loop is
Iron-Chromium (16-25%) – Nickel (7-20%)
Austenitic structure (FCC γ ) remains austenitic
at all temperature due to nickel.
Better corrosion resistance than other steels.
Used for chemical equipment, pressure vessels
Alloying element, columbium, prevents
intergranular corrosion if the alloy is to be used
General Properties: Contains 2-4% Carbon and 13% Si.
• Easily melted, very fluid, low shrinkage, easily
• Low impact resistance and ductility.
• Types of Cast Iron:
White cast iron
Gray cast iron
Malleable cast iron
Ductile cast iron
White Cast iron
Much of Carbon forms Iron Carbide instead of
graphite up on solidification.
• Fractured surface appears white and crystalline.
• Low carbon (2.5 – 3%) and silicon (0.5 – 1.5%)
• Excellent wear resistance.
Courtesy of central Foundry
Gray Cast Iron
Carbon exceeds the amount that can dissolve in
austenite and precipitate as graphite flakes.
• Fractured surface appears gray.
• Excellent machinability, hardness and wear resistance,
and vibration damping capacity.
• 2.5 – 4% C and 1 – 3% Si (Promotes formation of
After “Metals Handbook,” vol. 7, 8th ed., American Society for Metals, 1972, p.82.
Ductile Cast iron
Has processing advantages of cast iron and
engineering advantages of steel.
Good fluidity, castability, machinability, and wear
High strength, toughness, ductility and hardenability
(due to spherical nodules of graphite).
3-4% C and 1.8 – 2.8 % Si and low impurities.
Bull’s eye type microstructure.
After “Metals Handbook,” vol. 7, 8th ed., American Society for Metals, 1972, p.88.
Malleable Cast Iron
2-2.6 % C and 1.1 – 1.6% Si.
White cast iron is heated in malleablizing furnace to
dislocate carbide into graphite.
• Irregular nodules of graphite are formed.
• Good castability, machinability, moderate strength,
toughness and uniformity.
After “Metals Handbook,” vol. 7, 8th ed., American Society for Metals, 1972, p.95.
Heat treatment of white irons to produce malleable irons
Graphitization: Castings heated above the eutectoid
temperature (9400C) and held for 3 to 20h depending on
the composition and structure.
graphite and austenite.
• Ferritic malleable iron: Fast cooled from 740-7600C and
then slowly cooled.
• Pearlitic malleable iron: Slowly cooled up to 8700C and
then air cooled.
• Tempered martensitic malleable iron: Casting cooled in
furnace to a quenching temperature and homogenized and
then quenched in agitated oil.
Magnesium, Titanium and Nickel Alloys
Low density metal, high cost, low castability, low
strength, poor creep, fatigue and wear resistance.
Two types: wrought alloys (sheet, plate, extrusion)
and casting alloys (casting).
Designated by two capital letters and two or three
First two letters indicate two major alloying
The numbers indicate wt% of alloying elements.
Structure and Properties of Magnesium Alloys
• Limited cold working due to HCP structure.
• Usually hot worked.
• Al and Zn are added to increase strength.
• Alloying with rare earth elements (cerium)
produces rigid boundary network.
• Tensile strength 179 – 310 MPa.
• Elongation – 2 to 11%
Low density and high strength
Expensive – used for aircraft applications.
Superior corrosion resistance.
Special technique needed to work with metal.
HCP at room temperature. Transforms to BCC
• Al and O increase transformation temperature.
• Tensile strength – 662 to 862 MPa
Expensive, good corrosion resistance and high
Commercial Nickel and Monel alloys: good weldability,
electrical conductivity and corrosion resistance.
Nickel + 32% Cu
Monel alloy (strengthens nickel).
Nickel based super alloys: High temperature creep
resistance and oxidizing resistance for gas turbine parts.
50 -60 % Ni + 15-20% Cr + 15-20% Co + 1-4% Al + 24% Ti.
3 phases – Gamma austenite, gamma prime, carbide
Unique combination of properties
Examples: Nickel aluminide
• Low density, good high temperature strength, less
corrosion but brittle.
• 0.1 % Boron and 6-9 % Cr added to reduce
embrittlement and to increase ductility.
• Applications : Jet engine, pistons, furnace parts,
magnetic applications (Fe3Si) and electronic
Shape Memory Alloys (SMA)
• SMA recover predefined shape when subjected to
appropriate heat treatment.
• Recovers strain and exerts forces
• Examples: AuCd, Cu-Zn-Al, Cu-Al-Ni, Ni-Ti
• Processed using hot and cold forming techniques and
heat treated at 500-800 0C at desired shape.
• At high temperature ---Regular cubic microstructure
• After cooling – Highly twinned platelets (Martensite)
Shape Memory Effect
SMA easily deformed in martensite state due to twin
boundaries and deformation is not recovered after load
• Heating causes Martensite
transformation so shape is recovered.
• Effect takes place over a range of temperature.
SMA - Hysterisis
Heating and cooling temperatures do not overlap –
• Applied stress may deform and transform SMA to
martensite – stress induced transformation
• Shape is recovered when stress is released
• Nitonol (NiTi) is commonly used SMA
Shape memory strain of 8.5%
Non-magnetic, corrosion resistant
• Applications: Vascular stents
Coffeepot thermostats, eyeglass
frames orthodontics, vibration
damper surgical tools
• Atoms arranged in random manner in metals under
• Produced by rapid quenching (10 5 K/s) – No time to
• Till now only small pieces could be produced
• No dislocation activity : Very hard, perfectly plastic,
high dimensional accuracy (no shrinkage)
Biomedical Applications: Biometals
Biometals come in direct contact with human body fluids.
Used to replace tissue
Support damaged tissue while heeling
• Biocompatibility : Internal environment of human body is
Metals degrade and release harmful ions
Chemical stability, corrosion resistance, non-carcinogenity and
non-toxicity is called biocompatibility.
High fatigue strength is desired.
Pt, Ti, Zr have good biocompatibility.
Co, Cu, Ni are toxic
Stainless Steels as Biometals
316 L stainless steel (cold worked, grain size of
minimum 5) is used most often
• Inexpensive, easily shaped
• limited corrosion resistance
inside the body
removed after healing
Used as bone screws
Cobalt Based Alloys
Cr promotes long term
Ni and W improve machinability
• Initially hot worked and then cold finished
• Used in permanent fixation devices
Total knee replacement
• Easily formed, outstanding corrosion resistance
• Low elastic modulus, highly biocompatible
• Pure Ti is used in low strength applications
• Alpha-beta alloys of Ti like Ti-6Al-4V (F1472)
are strengthened by solution heat treatment.
• Poor wear resistance and notch sensitivity
• Beta alloys have low elastic modulus
• Ion implantation improves wear resistance
Issues in Orthopaedic Applications
High yield strength, fatigue strength and hardness of
implants is desired.
Implant should support healing bone
• Low elastic modulus is desired
Implant and bone should carry proportionate amount of load
Implant should not shield the bone from load
Stress shielding stops remodeling of bone and weakens it.
Elastic modulus of bone is only 17 GPa while most alloys have
elastic modulus greater than 100 GPa.
Wear causes metallic toxicity
Co-Cr alloys have good wear resistance